#------------------------------------------------------------------------------
#$Date: 2020-12-09 03:53:15 +0200 (Wed, 09 Dec 2020) $
#$Revision: 259672 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/12/75/7127520.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7127520
loop_
_publ_author_name
'Li, Shaobin'
'Tan, Xiaoguo'
'Yue, Ming'
'Zhang, Li'
'Chai, Dongfeng'
'Wang, Wendi'
'Pan, Hong'
'Fan, Linlin'
'Zhao, Chunyan'
_publ_section_title
;
 A polyoxometalate-encapsulated nanocage cluster organic framework built
 from {Cu₄P₂} units and its efficient bifunctional
 electrochemical performance.
;
_journal_issue                   96
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              15177
_journal_page_last               15180
_journal_paper_doi               10.1039/d0cc06665f
_journal_volume                  56
_journal_year                    2020
_chemical_formula_sum            'C60 H57 Cu4 Mo12 N16 O50 P3'
_chemical_formula_weight         3300.55
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-09-26 deposited with the CCDC.	2020-11-09 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 105.586(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   24.841(6)
_cell_length_b                   18.316(4)
_cell_length_c                   10.897(5)
_cell_measurement_reflns_used    2367
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.30
_cell_measurement_theta_min      2.20
_cell_volume                     4776(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0828
_diffrn_reflns_av_unetI/netI     0.0821
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            13369
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.024
_diffrn_reflns_theta_max         25.024
_diffrn_reflns_theta_min         1.400
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    2.538
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.290
_exptl_crystal_description       block
_exptl_crystal_F_000             3174
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_exptl_transmission_factor_max   0.776
_exptl_transmission_factor_min   0.701
_refine_diff_density_max         2.799
_refine_diff_density_min         -1.092
_refine_diff_density_rms         0.221
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.769
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     360
_refine_ls_number_reflns         4363
_refine_ls_number_restraints     36
_refine_ls_restrained_S_all      0.790
_refine_ls_R_factor_all          0.1046
_refine_ls_R_factor_gt           0.0617
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.2000P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1834
_refine_ls_wR_factor_ref         0.2170
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2789
_reflns_number_total             4365
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0cc06665f2.cif
_cod_data_source_block           LL
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_original_formula_sum        'C60 H57  Cu4 Mo12 N16 O50 P3'
_cod_database_code               7127520
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.701
_shelx_estimated_absorpt_t_max   0.776
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo -0.06811(5) 0.09866(5) 0.20528(10) 0.0475(3) Uani 1 1 d . . . . .
Mo2 Mo 0.12826(4) -0.09933(5) 0.13711(10) 0.0489(3) Uani 1 1 d . . . . .
Mo4 Mo 0.000000 0.19693(7) 0.000000 0.0568(5) Uani 1 2 d S T P . .
Mo3 Mo 0.06061(5) 0.000000 0.34215(12) 0.0447(4) Uani 1 2 d S T P . .
Cu1 Cu 0.00403(4) 0.40698(6) 0.18629(11) 0.0268(3) Uani 1 1 d . . . . .
P1 P 0.000000 0.000000 0.000000 0.0269(10) Uani 1 4 d S T P . .
P2 P 0.07550(11) 0.500000 0.0450(3) 0.0223(7) Uani 1 2 d S T P . .
O3 O 0.0391(5) -0.0676(6) -0.0130(11) 0.026(3) Uani 0.5 1 d . . P . .
O9 O 0.0014(3) 0.0730(4) 0.3203(10) 0.069(3) Uani 1 1 d . . . . .
O4 O 0.0726(5) -0.1766(6) 0.1090(9) 0.099(3) Uani 1 1 d . U . . .
O14 O 0.000000 0.2894(5) 0.000000 0.040(2) Uani 1 2 d S T P . .
O13 O -0.0308(5) 0.1777(6) 0.1416(9) 0.098(3) Uani 1 1 d . U . . .
O12 O -0.0995(4) 0.1456(5) 0.2998(9) 0.068(2) Uani 1 1 d . . . . .
O10 O -0.0926(4) 0.000000 0.2184(14) 0.062(4) Uani 1 2 d S T P . .
O11 O -0.1233(5) 0.1037(5) 0.0411(9) 0.092(3) Uani 1 1 d . U . . .
O8 O 0.0885(8) 0.000000 0.4966(13) 0.116(7) Uani 1 2 d S T P . .
O7 O 0.1054(3) -0.0722(4) 0.2877(10) 0.065(2) Uani 1 1 d . . . . .
O5 O 0.1543(5) 0.000000 0.1381(13) 0.064(4) Uani 1 2 d S T P . .
O6 O 0.1888(4) -0.1433(5) 0.2026(9) 0.078(3) Uani 1 1 d . . . . .
O16 O 0.0660(2) 0.4290(3) 0.1135(6) 0.0265(13) Uani 1 1 d . U . . .
O17 O -0.0386(3) 0.500000 0.0990(8) 0.0255(19) Uani 1 2 d S T P . .
N1 N -0.0664(3) 0.3656(4) 0.2122(7) 0.0297(17) Uani 1 1 d . . . . .
N2 N -0.1517(3) 0.3166(4) 0.1551(8) 0.0317(18) Uani 1 1 d . . . . .
N3 N 0.0527(3) 0.3298(4) 0.2949(7) 0.0279(17) Uani 1 1 d . . . . .
N4 N 0.1327(3) 0.2753(4) 0.3997(8) 0.0324(18) Uani 1 1 d . . . . .
C1 C -0.0889(4) 0.3724(6) 0.3140(10) 0.042(3) Uani 1 1 d . . . . .
H1 H -0.071236 0.392531 0.392910 0.051 Uiso 1 1 calc R U . . .
C2 C -0.1049(3) 0.3332(5) 0.1165(9) 0.031(2) Uani 1 1 d . . . . .
H2 H -0.100341 0.323582 0.036071 0.037 Uiso 1 1 calc R U . . .
C3 C -0.1434(4) 0.3435(6) 0.2774(10) 0.044(3) Uani 1 1 d . . . . .
H3 H -0.168971 0.342744 0.326053 0.053 Uiso 1 1 calc R U . . .
C4 C -0.2023(3) 0.2829(5) 0.0763(10) 0.033(2) Uani 1 1 d . . . . .
C5 C -0.2277(4) 0.2256(6) 0.1273(11) 0.044(3) Uani 1 1 d . . . . .
H5 H -0.212684 0.209482 0.210391 0.052 Uiso 1 1 calc R U . . .
C6 C -0.2241(4) 0.3061(6) -0.0496(10) 0.042(2) Uani 1 1 d . . . . .
H6 H -0.206250 0.343176 -0.081868 0.050 Uiso 1 1 calc R U . . .
C7 C 0.0405(4) 0.2711(5) 0.3683(9) 0.034(2) Uani 1 1 d . . . . .
H7 H 0.004767 0.257505 0.370933 0.040 Uiso 1 1 calc R U . . .
C8 C 0.0878(4) 0.2378(5) 0.4335(10) 0.035(2) Uani 1 1 d . . . . .
H8 H 0.090865 0.198521 0.489068 0.042 Uiso 1 1 calc R U . . .
C9 C 0.1084(4) 0.3291(5) 0.3185(9) 0.032(2) Uani 1 1 d . . . . .
H9 H 0.128336 0.362152 0.282876 0.038 Uiso 1 1 calc R U . . .
C10 C 0.1933(4) 0.2629(5) 0.4501(9) 0.034(2) Uani 1 1 d . . . . .
C11 C 0.2305(4) 0.3191(6) 0.4557(11) 0.044(3) Uani 1 1 d . . . . .
H11 H 0.217273 0.365080 0.426133 0.052 Uiso 1 1 calc R U . . .
C12 C 0.2121(4) 0.1917(6) 0.4949(10) 0.041(2) Uani 1 1 d . . . . .
H12 H 0.186891 0.153675 0.491254 0.049 Uiso 1 1 calc R U . . .
C14 C 0.1500(4) 0.500000 0.0496(13) 0.025(3) Uani 1 2 d S T P . .
C15 C 0.1898(5) 0.500000 0.1716(13) 0.035(3) Uani 1 2 d S T P . .
H15 H 0.177775 0.500000 0.245441 0.042 Uiso 1 2 calc R U P . .
C16 C 0.2475(6) 0.500000 0.1794(16) 0.046(4) Uani 1 2 d S TU P . .
H16 H 0.273948 0.500000 0.258165 0.055 Uiso 1 2 calc R U P . .
C17 C 0.2645(5) 0.500000 0.0647(15) 0.040(3) Uani 1 2 d S TU P . .
H17 H 0.302434 0.500000 0.069371 0.048 Uiso 1 2 calc R U P . .
C18 C 0.2264(5) 0.500000 -0.0526(17) 0.046(4) Uani 1 2 d S T P . .
H18 H 0.238695 0.500000 -0.126010 0.055 Uiso 1 2 calc R U P . .
C13 C 0.1696(5) 0.500000 -0.0622(14) 0.031(3) Uani 1 2 d S T P . .
H13 H 0.144051 0.500000 -0.142180 0.038 Uiso 1 2 calc R U P . .
O1 O 0.0499(7) 0.000000 0.1095(17) 0.029(4) Uani 0.5 2 d S T P . .
O2 O -0.0087(6) 0.000000 0.1336(17) 0.028(4) Uani 0.5 2 d S T P . .
O1W O 0.1558(8) 0.500000 0.500(2) 0.166(10) Uani 1 2 d S T P . .
O15 O 0.0259(2) 0.500000 0.3924(6) 0.0069(13) Uiso 1 2 d S . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O12 Mo1 O11 102.2(5) . . ?
O12 Mo1 O9 102.1(4) . . ?
O11 Mo1 O9 155.6(5) . . ?
O12 Mo1 O10 103.1(5) . . ?
O11 Mo1 O10 87.4(5) . . ?
O9 Mo1 O10 88.2(4) . . ?
O12 Mo1 O13 100.5(5) . . ?
O11 Mo1 O13 85.5(4) . . ?
O9 Mo1 O13 89.0(4) . . ?
O10 Mo1 O13 156.3(5) . . ?
O12 Mo1 O3 158.2(4) . 5 ?
O11 Mo1 O3 61.4(5) . 5 ?
O9 Mo1 O3 94.7(4) . 5 ?
O10 Mo1 O3 91.0(5) . 5 ?
O13 Mo1 O3 65.8(4) . 5 ?
O12 Mo1 O2 159.6(5) . . ?
O11 Mo1 O2 94.2(5) . . ?
O9 Mo1 O2 62.3(5) . . ?
O10 Mo1 O2 65.4(4) . . ?
O13 Mo1 O2 92.7(5) . . ?
O3 Mo1 O2 42.1(4) 5 . ?
O6 Mo2 O7 101.3(4) . . ?
O6 Mo2 O11 102.5(5) . 5 ?
O7 Mo2 O11 156.2(5) . 5 ?
O6 Mo2 O5 100.8(5) . . ?
O7 Mo2 O5 85.9(4) . . ?
O11 Mo2 O5 88.6(5) 5 . ?
O6 Mo2 O4 103.6(5) . . ?
O7 Mo2 O4 87.8(4) . . ?
O11 Mo2 O4 87.7(4) 5 . ?
O5 Mo2 O4 155.5(5) . . ?
O6 Mo2 O3 160.4(4) . . ?
O7 Mo2 O3 95.0(4) . . ?
O11 Mo2 O3 62.0(5) 5 . ?
O5 Mo2 O3 91.3(5) . . ?
O4 Mo2 O3 65.7(4) . . ?
O6 Mo2 O1 158.5(5) . . ?
O7 Mo2 O1 62.7(5) . . ?
O11 Mo2 O1 93.9(5) 5 . ?
O5 Mo2 O1 65.4(4) . . ?
O4 Mo2 O1 90.7(5) . . ?
O3 Mo2 O1 41.1(4) . . ?
O14 Mo4 O4 101.3(3) . 5 ?
O14 Mo4 O4 101.3(3) . 6 ?
O4 Mo4 O4 157.5(7) 5 6 ?
O14 Mo4 O13 100.5(3) . 2 ?
O4 Mo4 O13 88.7(5) 5 2 ?
O4 Mo4 O13 87.2(4) 6 2 ?
O14 Mo4 O13 100.5(3) . . ?
O4 Mo4 O13 87.2(4) 5 . ?
O4 Mo4 O13 88.7(5) 6 . ?
O13 Mo4 O13 158.9(7) 2 . ?
O14 Mo4 O3 156.7(3) . 5 ?
O4 Mo4 O3 63.1(4) 5 5 ?
O4 Mo4 O3 95.3(4) 6 5 ?
O13 Mo4 O3 96.4(4) 2 5 ?
O13 Mo4 O3 63.4(4) . 5 ?
O14 Mo4 O3 156.7(3) . 6 ?
O4 Mo4 O3 95.3(4) 5 6 ?
O4 Mo4 O3 63.1(4) 6 6 ?
O13 Mo4 O3 63.4(4) 2 6 ?
O13 Mo4 O3 96.4(4) . 6 ?
O3 Mo4 O3 46.5(5) 5 6 ?
O8 Mo3 O7 101.4(6) . . ?
O8 Mo3 O7 101.4(6) . 6 ?
O7 Mo3 O7 87.0(4) . 6 ?
O8 Mo3 O9 102.8(6) . 6 ?
O7 Mo3 O9 88.3(3) . 6 ?
O7 Mo3 O9 155.8(4) 6 6 ?
O8 Mo3 O9 102.8(6) . . ?
O7 Mo3 O9 155.8(4) . . ?
O7 Mo3 O9 88.3(3) 6 . ?
O9 Mo3 O9 86.3(4) 6 . ?
O8 Mo3 O1 161.9(8) . . ?
O7 Mo3 O1 66.2(4) . . ?
O7 Mo3 O1 66.2(4) 6 . ?
O9 Mo3 O1 90.3(4) 6 . ?
O9 Mo3 O1 90.3(4) . . ?
O8 Mo3 O2 161.5(8) . . ?
O7 Mo3 O2 92.0(4) . . ?
O7 Mo3 O2 92.0(4) 6 . ?
O9 Mo3 O2 64.5(4) 6 . ?
O9 Mo3 O2 64.5(4) . . ?
O1 Mo3 O2 36.6(5) . . ?
O16 Cu1 N1 162.2(3) . . ?
O16 Cu1 N3 88.2(3) . . ?
N1 Cu1 N3 93.5(3) . . ?
O16 Cu1 O17 90.3(3) . . ?
N1 Cu1 O17 91.0(3) . . ?
N3 Cu1 O17 169.7(3) . . ?
O16 Cu1 Cu1 78.09(17) . 6_565 ?
N1 Cu1 Cu1 112.3(2) . 6_565 ?
N3 Cu1 Cu1 134.3(2) . 6_565 ?
O17 Cu1 Cu1 35.56(17) . 6_565 ?
O1 P1 O1 180.0 5 . ?
O1 P1 O2 62.1(9) 5 5 ?
O1 P1 O2 117.9(9) . 5 ?
O1 P1 O2 117.9(9) 5 . ?
O1 P1 O2 62.1(9) . . ?
O2 P1 O2 180.0 5 . ?
O1 P1 O3 109.0(6) 5 . ?
O1 P1 O3 71.0(6) . . ?
O2 P1 O3 70.8(5) 5 . ?
O2 P1 O3 109.2(5) . . ?
O1 P1 O3 71.0(6) 5 2 ?
O1 P1 O3 109.0(6) . 2 ?
O2 P1 O3 109.2(5) 5 2 ?
O2 P1 O3 70.8(5) . 2 ?
O3 P1 O3 78.9(8) . 2 ?
O1 P1 O3 109.0(6) 5 6 ?
O1 P1 O3 71.0(6) . 6 ?
O2 P1 O3 70.8(5) 5 6 ?
O2 P1 O3 109.2(5) . 6 ?
O3 P1 O3 101.1(8) . 6 ?
O3 P1 O3 180.0(10) 2 6 ?
O1 P1 O3 71.0(6) 5 5 ?
O1 P1 O3 109.0(6) . 5 ?
O2 P1 O3 109.2(5) 5 5 ?
O2 P1 O3 70.8(5) . 5 ?
O3 P1 O3 180.0 . 5 ?
O3 P1 O3 101.1(8) 2 5 ?
O3 P1 O3 78.9(8) 6 5 ?
O16 P2 O16 114.2(5) . 6_565 ?
O16 P2 O17 110.7(3) . 5_565 ?
O16 P2 O17 110.7(3) 6_565 5_565 ?
O16 P2 C14 105.7(3) . . ?
O16 P2 C14 105.7(3) 6_565 . ?
O17 P2 C14 109.7(5) 5_565 . ?
P1 O3 O2 52.6(6) . 5 ?
P1 O3 O1 51.1(6) . . ?
O2 O3 O1 91.0(8) 5 . ?
P1 O3 Mo1 125.3(6) . 5 ?
O2 O3 Mo1 72.6(6) 5 5 ?
O1 O3 Mo1 141.0(8) . 5 ?
P1 O3 Mo2 125.9(6) . . ?
O2 O3 Mo2 140.5(7) 5 . ?
O1 O3 Mo2 74.8(6) . . ?
Mo1 O3 Mo2 95.4(4) 5 . ?
P1 O3 Mo4 117.3(6) . 5 ?
O2 O3 Mo4 125.3(7) 5 5 ?
O1 O3 Mo4 125.3(7) . 5 ?
Mo1 O3 Mo4 92.0(4) 5 5 ?
Mo2 O3 Mo4 91.8(4) . 5 ?
Mo1 O9 Mo3 140.4(5) . . ?
Mo4 O4 Mo2 138.8(6) 5 . ?
Mo4 O13 Mo1 138.7(6) . . ?
Mo1 O10 Mo1 139.8(6) 6 . ?
Mo1 O11 Mo2 140.4(7) . 5 ?
Mo2 O7 Mo3 139.7(5) . . ?
Mo2 O5 Mo2 141.0(6) 6 . ?
P2 O16 Cu1 127.4(3) . . ?
P2 O17 Cu1 122.4(2) 5_565 . ?
P2 O17 Cu1 122.4(2) 5_565 6_565 ?
Cu1 O17 Cu1 108.9(3) . 6_565 ?
C2 N1 C1 107.9(8) . . ?
C2 N1 Cu1 121.6(6) . . ?
C1 N1 Cu1 129.9(6) . . ?
C2 N2 C3 107.2(7) . . ?
C2 N2 C4 125.6(8) . . ?
C3 N2 C4 126.9(8) . . ?
C9 N3 C7 104.5(7) . . ?
C9 N3 Cu1 123.0(6) . . ?
C7 N3 Cu1 132.4(6) . . ?
C9 N4 C8 105.9(7) . . ?
C9 N4 C10 126.0(8) . . ?
C8 N4 C10 127.9(8) . . ?
N1 C1 C3 107.8(9) . . ?
N1 C1 H1 126.1 . . ?
C3 C1 H1 126.1 . . ?
N1 C2 N2 110.1(8) . . ?
N1 C2 H2 124.9 . . ?
N2 C2 H2 124.9 . . ?
N2 C3 C1 106.9(9) . . ?
N2 C3 H3 126.6 . . ?
C1 C3 H3 126.6 . . ?
C6 C4 N2 119.7(8) . . ?
C6 C4 C5 121.0(8) . . ?
N2 C4 C5 119.3(9) . . ?
C6 C5 C4 118.2(10) 7_455 . ?
C6 C5 H5 120.9 7_455 . ?
C4 C5 H5 120.9 . . ?
C5 C6 C4 120.8(9) 7_455 . ?
C5 C6 H6 119.6 7_455 . ?
C4 C6 H6 119.6 . . ?
C8 C7 N3 110.6(8) . . ?
C8 C7 H7 124.7 . . ?
N3 C7 H7 124.7 . . ?
C7 C8 N4 106.0(8) . . ?
C7 C8 H8 127.0 . . ?
N4 C8 H8 127.0 . . ?
N3 C9 N4 113.0(8) . . ?
N3 C9 H9 123.5 . . ?
N4 C9 H9 123.5 . . ?
C11 C10 C12 121.0(8) . . ?
C11 C10 N4 120.6(8) . . ?
C12 C10 N4 118.5(8) . . ?
C10 C11 C12 121.1(9) . 7_556 ?
C10 C11 H11 119.4 . . ?
C12 C11 H11 119.4 7_556 . ?
C11 C12 C10 117.9(9) 7_556 . ?
C11 C12 H12 121.0 7_556 . ?
C10 C12 H12 121.0 . . ?
C15 C14 C13 119.1(11) . . ?
C15 C14 P2 117.7(10) . . ?
C13 C14 P2 123.2(10) . . ?
C14 C15 C16 119.5(14) . . ?
C14 C15 H15 120.2 . . ?
C16 C15 H15 120.2 . . ?
C17 C16 C15 118.9(14) . . ?
C17 C16 H16 120.6 . . ?
C15 C16 H16 120.6 . . ?
C18 C17 C16 121.7(12) . . ?
C18 C17 H17 119.1 . . ?
C16 C17 H17 119.1 . . ?
C17 C18 C13 120.3(14) . . ?
C17 C18 H18 119.9 . . ?
C13 C18 H18 119.9 . . ?
C18 C13 C14 120.5(13) . . ?
C18 C13 H13 119.7 . . ?
C14 C13 H13 119.7 . . ?
P1 O1 O2 60.8(9) . . ?
P1 O1 O3 58.0(6) . 6 ?
O2 O1 O3 99.6(9) . 6 ?
P1 O1 O3 58.0(6) . . ?
O2 O1 O3 99.6(9) . . ?
O3 O1 O3 87.7(11) 6 . ?
P1 O1 Mo3 131.7(10) . . ?
O2 O1 Mo3 71.0(9) . . ?
O3 O1 Mo3 135.9(6) 6 . ?
O3 O1 Mo3 135.9(6) . . ?
P1 O1 Mo2 122.0(6) . 6 ?
O2 O1 Mo2 133.2(5) . 6 ?
O3 O1 Mo2 64.1(5) 6 6 ?
O3 O1 Mo2 121.6(9) . 6 ?
Mo3 O1 Mo2 90.6(5) . 6 ?
P1 O1 Mo2 122.0(6) . . ?
O2 O1 Mo2 133.2(5) . . ?
O3 O1 Mo2 121.6(9) 6 . ?
O3 O1 Mo2 64.1(5) . . ?
Mo3 O1 Mo2 90.6(5) . . ?
Mo2 O1 Mo2 87.9(5) 6 . ?
P1 O2 O1 57.2(9) . . ?
P1 O2 O3 56.5(6) . 2 ?
O1 O2 O3 96.0(9) . 2 ?
P1 O2 O3 56.5(6) . 5 ?
O1 O2 O3 96.0(9) . 5 ?
O3 O2 O3 86.0(11) 2 5 ?
P1 O2 Mo3 129.6(8) . . ?
O1 O2 Mo3 72.5(9) . . ?
O3 O2 Mo3 136.2(5) 2 . ?
O3 O2 Mo3 136.2(5) 5 . ?
P1 O2 Mo1 121.8(6) . 6 ?
O1 O2 Mo1 133.7(4) . 6 ?
O3 O2 Mo1 65.3(4) 2 6 ?
O3 O2 Mo1 122.4(8) 5 6 ?
Mo3 O2 Mo1 92.0(5) . 6 ?
P1 O2 Mo1 121.8(6) . . ?
O1 O2 Mo1 133.7(4) . . ?
O3 O2 Mo1 122.4(8) 2 . ?
O3 O2 Mo1 65.3(4) 5 . ?
Mo3 O2 Mo1 92.0(5) . . ?
Mo1 O2 Mo1 88.8(5) 6 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O12 1.685(8) . ?
Mo1 O11 1.941(10) . ?
Mo1 O9 1.899(9) . ?
Mo1 O10 1.924(4) . ?
Mo1 O13 1.945(9) . ?
Mo1 O3 2.458(11) 5 ?
Mo1 O2 2.583(11) . ?
Mo2 O6 1.686(8) . ?
Mo2 O7 1.941(9) . ?
Mo2 O11 1.914(10) 5 ?
Mo2 O5 1.930(4) . ?
Mo2 O4 1.944(9) . ?
Mo2 O3 2.444(11) . ?
Mo2 O1 2.622(12) . ?
Mo4 O14 1.695(9) . ?
Mo4 O4 1.910(10) 5 ?
Mo4 O4 1.910(10) 6 ?
Mo4 O13 1.929(10) 2 ?
Mo4 O13 1.929(10) . ?
Mo4 O3 2.578(11) 5 ?
Mo4 O3 2.578(11) 6 ?
Mo3 O8 1.639(13) . ?
Mo3 O7 1.921(8) . ?
Mo3 O7 1.921(8) 6 ?
Mo3 O9 1.955(7) 6 ?
Mo3 O9 1.955(7) . ?
Mo3 O1 2.477(18) . ?
Mo3 O2 2.456(17) . ?
Cu1 O16 1.953(6) . ?
Cu1 N1 1.995(7) . ?
Cu1 N3 2.023(7) . ?
Cu1 O17 2.094(5) . ?
Cu1 Cu1 3.408(2) 6_565 ?
P1 O1 1.472(17) 5 ?
P1 O1 1.472(17) . ?
P1 O2 1.528(17) 5 ?
P1 O2 1.528(17) . ?
P1 O3 1.603(12) . ?
P1 O3 1.604(12) 2 ?
P1 O3 1.604(12) 6 ?
P1 O3 1.604(12) 5 ?
P2 O16 1.549(6) . ?
P2 O16 1.550(6) 6_565 ?
P2 O17 1.591(9) 5_565 ?
P2 C14 1.839(11) . ?
O3 O2 1.815(17) 5 ?
O3 O1 1.788(18) . ?
N1 C2 1.348(11) . ?
N1 C1 1.375(13) . ?
N2 C2 1.374(11) . ?
N2 C3 1.384(13) . ?
N2 C4 1.454(11) . ?
N3 C9 1.337(11) . ?
N3 C7 1.422(11) . ?
N4 C9 1.353(11) . ?
N4 C8 1.441(12) . ?
N4 C10 1.473(11) . ?
C1 C3 1.409(12) . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 C6 1.400(14) . ?
C4 C5 1.413(13) . ?
C5 C6 1.393(13) 7_455 ?
C5 H5 0.9300 . ?
C6 H6 0.9300 . ?
C7 C8 1.344(13) . ?
C7 H7 0.9300 . ?
C8 H8 0.9300 . ?
C9 H9 0.9300 . ?
C10 C11 1.375(14) . ?
C10 C12 1.426(13) . ?
C11 C12 1.397(13) 7_556 ?
C11 H11 0.9300 . ?
C12 H12 0.9300 . ?
C14 C15 1.427(17) . ?
C14 C13 1.428(18) . ?
C15 C16 1.414(19) . ?
C15 H15 0.9300 . ?
C16 C17 1.42(2) . ?
C16 H16 0.9300 . ?
C17 C18 1.37(2) . ?
C17 H17 0.9300 . ?
C18 C13 1.386(18) . ?
C18 H18 0.9300 . ?
C13 H13 0.9300 . ?
O1 O2 1.55(2) . ?
